Enhanced light absorption of amorphous silicon thin film by substrate control and ion irradiation
© Yuan et al.; licensee Springer. 2014
Received: 18 January 2014
Accepted: 30 March 2014
Published: 9 April 2014
Large-area periodically aligned silicon nanopillar (PASiNP) arrays were fabricated by magnetic sputtering with glancing angle deposition (GLAD) on substrates coated by a monolayer of close-packed polystyrene (PS) nanospheres. The structure of PASiNP arrays could be manipulated by changing the diameter of PS nanospheres. Enhanced light absorptance within a wavelength range from 300 to 1,000 nm was observed as the diameter of nanopillars and porosity of PASiNP arrays increased. Meanwhile, Xe ion irradiation with dose from 1 × 1014 to 50 × 1014 ions/cm2 was employed to modify the surface morphology and top structure of thin films, and the effect of the irradiation on the optical bandgap was discussed.
81.15.Cd; 78.66.Jg; 61.80.Jh
KeywordsEnhanced light absorption Silicon Irridiation
With the development of society, problems of energy crisis and environment pollution have been of further concern. In order to maintain sustainable growth, a clean and renewable energy source is urgently required. Among all new types of energy sources, solar energy is the most promising one for it is safe, cheap, inexhaustible, and environment-friendly.
In 1976, Carlson and Wronski  invented a new type of thin film solar cell that utilized amorphous silicon (a-Si) deposited from a glow discharge in silane (SiH4) and achieved a power conversion efficiency of 2.4% in AM-1 sunlight. After that, silicon thin film solar cells have been widely investigated in different ways and methods . Compared with conventional solar cell, amorphous silicon thin film solar cell is low cost and could be deposited on various substrates such as glass, stainless steel, ceramic plate, and plastic .
Studies focused on textured surface showed that it can improve absorption by reducing reflection. Textured surface can be conventionally obtained by either dry or wet ion etching [4–7]. In 2011, Wong and Yu  simulated a nanopillar-array-textured surface and came to a conclusion that it may enhance light absorption and increase the efficiency of the silicon-based solar cell.
The effects of low-energy heavy ion irradiation on silicon thin film have been systematically studied during the past 50 years. During the irradiation, some traditional defects were generated; however, latent tracks, amorphous transition, or other special effects were not observed [9, 10]. Enhanced light absorption was obtained in works on n-type crystal silicon irradiated by high-energy Xe ion , which provided a promising method for the modification of amorphous silicon thin film.
In this research, we coated a polystyrene (PS) sphere monolayer on glass substrate and fabricated silicon thin film via magnetic sputtering with glancing angle deposition (GLAD) in order to achieve periodically aligned silicon nanopillar (PASiNP) arrays. The influences of silicon nanopillar diameter and Xe ion irradiation on the light absorption of thin film were studied. The mechanism of ion irradiation was also discussed.
We replicate this nanostructure by magnetic sputtering deposition with its advantage of controllable fabrication, and an expected enhancement in light absorption was observed.
Glasses were first cut into squares of about 3 × 3 cm2 in size and then thoroughly cleaned with acetone in an ultrasonic bath for 20 min. After washing off the residual acetone by deionized water, they were cleaned with ethanol in an ultrasonic bath for another 20 min. The glasses were immersed in H2SO4-H2O2 solution (3:1, v/v) for 8 h and then cleaned with deionized water in an ultrasonic bath for 30 min and with NH3-H2O2-H2O solution (1:1:3, v/v) for another 30 min. After that, glasses with hydrophilic surfaces were obtained .
Details of spinning and drying
Diameter of PS nanosphere (nm)
Rate and time of spinning (r/min × min)
Rate and time of drying (r/min × min)
120 × 1
350 × 4
120 × 1
250 × 4
120 × 1
150 × 4
The silicon thin film was then deposited on the substrates via magnetic sputtering in argon atmosphere at 1.5 Pa for 90 min at a deposition angle of about 80°. The sputtering power was 90 W and the voltage was 0.5 kV.
Afterwards, films deposited on the 200-nm PS nanosphere monolayer were irradiated by 200-keV Xe ion with doses of 1 × 1014, 5 × 1014, 10 × 1014, and 50 × 1014 ion/cm2, in order to investigate its influence on the light absorption of thin film.
The morphology of films was observed by scanning electron microscopy (SEM). The X-ray diffraction (XRD) patterns were tested by Rigaku X-ray analytical instrument (Rigaku Corporation, Tokyo, Japan). The transmittance (T) and reflectance (R) spectra within the wavelength range from 300 to 1,000 nm were recorded by a UV-Vis-NIR spectrometer.
Results and discussion
After 90 min of deposition, films with thickness of about 700 nm were obtained, as shown in Figure 1. They were marked after their deposition time and the diameter of PS nanospheres as 90-0, 90-200, 90-500, and 90-1000; 0 represented the plain glass, which was used for comparison. For the films deposited on patterned substrates, owing to GLAD and shadowing effect, each nanosphere leads to the formation of one nanopillar. The size of nanopillars is determined by the diameter of the PS nanospheres beneath, and the nanopillar arrays replicate the close-packed pattern of the monolayer. Nanopillars separate from each other, and porosity rises as the diameter increases.
The film deposited on plain glass showed poor absorptance of lower than 10%, especially within a wavelength above 800 nm. In comparison, the absorptance of films deposited on patterned substrates enhances appreciably to more than 80%. As the diameter of the nanopillar increases, the absorptance of the corresponding film rises within the whole wavelength range. The positive correlation between absorptance and diameter can be attributed to the increasing porosity of the nanostructure, which extensively lengthens the path of incident light and enhances the absorptance .
The optical bandgap of thin films as deposited
E g (eV)
The reduction of optical bandgap is in accordance with the increase of absorptance. A material can only absorb photons with energy higher than its bandgap, so optical bandgap holds the essence of light absorption and the absorptance depends straightly on optical bandgap. The manipulation of optical bandgap would have direct influence on absorptance.
In the view of the original film shown in Figure 1b, silicon nanopillars are separated from each other. After ion irradiation, the top part of silicon nanopillars melted and recrystallized during the process. With the increasing of irradiation dose, the top part of the silicon nanopillars tends to connect with its neighbors, while the bottom part remains unaffected.
Optical bandgap after irradiation
Irradiation dose (1014ions/cm2)
E g (eV)
We prepared self-assembled monolayers of PS nanospheres and fabricated periodically aligned silicon nanopillar arrays by magnetic sputtering deposition. We improve the absorptance of thin film by changing the diameter of the silicon nanopillar. With the increase of the diameter of the nanopillar, optical bandgap decreases and absorptance increases.
The influence of Xe ion irradiation on the optical bandgap was also investigated. The bandgap decreases with the increase of irradiation dose. It may be induced by the recrystallization during the irradiation and lead to the change in grain size, which is closely related to the bandgap of the film.
All authors belong to the School of Materials Science and Engineering, Tsinghua University, People's Republic of China. FY is a master candidate interested in amorphous silicon thin film. ZL is an associate professor whose research fields include thin film material and nuclear material. TZ is a master candidate interested in the fabrication of nanostructure. WM is an associate professor working on nanostructure characterization. ZZ is the school dean professor with research interest in nanostructures and SERS effect.
glancing angle deposition
periodically aligned silicon nanopillar
scanning electron microscopy
The authors are grateful to the financial support by the National Natural Science Foundation of China (under Grants 61176003 and 61076003).
- Carlson DE, Wronski CR: Amorphous silicon solar cell. Appl Phys Lett 1976, 28(11):671. 10.1063/1.88617View Article
- Green MA, Emery K, Hishikawa Y, Warta W, Dunlop ED: Solar cell efficiency tables (version 39). Prog Photovolt Res Appl 2011, 20: 12.View Article
- Chopra KL, Paulson PD, Dutta V: Thin-film solar cells: an overview. Prog Photovolt Res Appl 2004, 12: 69. 10.1002/pip.541View Article
- Marty F, Rousseau L, Saadany B, Mercier B, Français O, Mita Y, Bourouina T: Advanced etching of silicon based on deep reactive ion etching for silicon high aspect ratio microstructures and three-dimensional micro- and nanostructures. Microelectron J 2005, 36: 673. 10.1016/j.mejo.2005.04.039View Article
- Koynov S, Brandt MS, Stutzmann M: Black nonreflecting silicon surfaces for solar cells. Appl Phys Lett 2006, 88: 203107. 10.1063/1.2204573View Article
- Huang MJ, Yang CR, Chiou YC, Lee RT: Fabrication of nanoporous antireflection surfaces on silicon. Sol Energy Mater Sol Cells 2008, 92: 1352. 10.1016/j.solmat.2008.05.014View Article
- Wu C, Crouch CH, Zhao L, Carey JE, Younkin R, Levinson JA, Mazur E, Farrell RM, Gothoskar P, Karger A: Near-unity below-band-gap absorption by microstructured silicon. Appl Phys Lett 1850, 2001: 78.
- Yu HY: Enhanced Si thin film solar cells short-circuit current with rational-designed Si nano-pillar array surface texturing. In SPIE/OSA/IEEE Asia Communications and Photonics. Shanghai: International Society for Optics and Photonics, November 2011; 2011:83120G.
- Mangiagalli P, Levalois M, Marie P, Rancoita PG, Rattaggi M: A comparative study of radiation damage on high resistivity silicon. EPJ Appl Phys 1999, 6: 121. 10.1051/epjap:1999161View Article
- Diao XG, Yoshida YU, Hayakawa K, Shimura F, Kambara T, Iwase A, Yano Y: Vacancy-oxygen complexes produced by 3.5 GeV Xe ion irradiation and their distribution along ion tracks in single-crystal silicon: an infrared study. J Phys: Condens Matter 2002, 14: L57. 10.1088/0953-8984/14/3/102
- Varichenko VS, Zaitsev AM, Kazutchits NM, Chelyadinskii AR, Penina NM, Martinovich VA, Latushko YI, Fahrner WR: Defect production in silicon irradiated with 5.68 GeV Xe ions. Nucl Instrum Methods Phys Res, Sect B 1996, 107: 268. 10.1016/0168-583X(95)01152-8View Article
- Li XC, Li JS, Chen T, Tay BK, Wang JX, Yu HY: Periodically aligned si nanopillar arrays as efficient antireflection layers for solar cell applications. Nanoscale Res Lett 2010, 5: 1721. 10.1007/s11671-010-9701-3View Article
- Chen ST, Li ZC, Zhang ZJ: Anisotropic TixSn1-xO2 nanostructures prepared by magnetron sputter deposition. Nanoscale Res Lett 2011, 6: 1.
- Su SM, Lin LH, Li ZC, Feng JY, Zhang ZJ: The fabrication of large-scale sub-10-nm core-shell silicon nanowire arrays. Nanoscale Res Lett 2013, 8: 1. 10.1186/1556-276X-8-1View Article
- Wood DL, Tauc JS: Weak absorption tails in amorphous semiconductors. Phys Rev B 1972, 5: 3144. 10.1103/PhysRevB.5.3144View Article
- Van Buuren T, Dinh LN, Chase LL, Siekhaus WJ, Terminello LJ: Changes in the electronic properties of Si nanocrystals as a function of particle size. Phys Rev Lett 1998, 80: 3803. 10.1103/PhysRevLett.80.3803View Article
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly credited.